* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
206 7.4.3 FOOD PACKAGING TECHNOLOGY PVdC coatings PVdC coatings may be modified to produce either a good heat-sealing polymer or a high-barrier polymer. There is a compromise to be made between the quality of sealing and the barrier properties required. Modification of the polymer to give a wider sealing range lowers the threshold for sealing to around 110Â°C at the expense of the gas barrier. PVdC coatings are applied to films and paper. The majority of general-purpose coatings supplied will have sealing properties starting to seal at 120Â°C and oxygen barrier of around 25 ml mâ2/24 h. For PET film, PVdC is normally chosen for high oxygen barrier (10 ml mâ2/24 h) and as a result may have poor sealing properties. The formulation needs to incorporate both silica and waxes as slip and antiblocking agents to prevent the coatings from sticking to the hot sealing surfaces. Typically, film producers apply coating weights of 3 g mâ2 or 2 Î¼m thickness. The specific gravity of PVdC is 1.3. Surface coatings can be applied to rigid containers such as the surface of PET beer bottles. 7.4.4 PVOH coatings With the environmental concern that dioxins may be produced if chlorinebased compounds are incinerated, an alternative high gas barrier has been sought to replace PVdC without needing to modify coating parameters. PVOH emulsions meet this requirement, but they are sensitive to moisture, losing barrier properties if the RH increases to more than 65% RH. Films with PVOH are therefore likely to be used as part of a laminate, with the PVOH on the inside of the web. BOPP with PVOH on the outside can be used, provided it is overlacquered with a protective varnish. PVOH also has no sealing properties. It is, however, an excellent surface to receive printing inks with low absorption or retention of solvents. Coating weights are similar to PVdC, but the specific gravity is nearer to 1.0 and film yield is slightly higher. 7.4.5 Low-temperature sealing coatings (LTSCs) LTSCs for OPP which seal at lower temperatures and have a wider sealing range are required to meet the demand for faster packaging machine speeds. These coatings, based on ionomer resins, applied in the form of emulsions are an alternative to both acrylic and PVdC coatings. As silica and waxes are likely to raise the sealing temperature threshold of any coatings, they are kept to a minimum with the consequence that friction is higher on LTSC than with the conventional coatings. The LTSC does not stick or block to PVdC or acrylic coatings and hence it is possible to have differentially coated films. The ionomer surface has good ink receptivity and does not retain printing ink solvents.